Upload
others
View
9
Download
0
Embed Size (px)
Citation preview
This content has been downloaded from IOPscience. Please scroll down to see the full text.
Download details:
IP Address: 130.74.117.167
This content was downloaded on 31/01/2014 at 19:16
Please note that terms and conditions apply.
Nanostructured graphene metasurface for tunable terahertz cloaking
View the table of contents for this issue, or go to the journal homepage for more
2013 New J. Phys. 15 123029
(http://iopscience.iop.org/1367-2630/15/12/123029)
Home Search Collections Journals About Contact us My IOPscience
Nanostructured graphene metasurface for tunableterahertz cloaking
Pai-Yen Chen1, Jason Soric1, Yashwanth R Padooru2,Hossein M Bernety2, Alexander B Yakovlev2 and Andrea Alu1,3
1 Department of Electrical and Computer Engineering, University of Texas atAustin, Austin, TX 78712, USA2 Center for Applied Electromagnetic Systems Research (CAESR), Departmentof Electrical Engineering, The University of Mississippi, University,MS 38677-1848, USAE-mail: [email protected]
New Journal of Physics 15 (2013) 123029 (12pp)Received 20 July 2013Published 17 December 2013Online at http://www.njp.org/doi:10.1088/1367-2630/15/12/123029
Abstract. We propose and analyze a graphene-based cloaking metasurfaceaimed at achieving widely tunable scattering cancelation in the terahertz (THz)spectrum. This ‘one-atom-thick’ mantle cloak is realized by means of a patternedmetasurface comprised of a periodic array of graphene patches, whose surfaceimpedance can be modeled with a simple yet accurate analytical expression.By adjusting the geometry and Fermi energy of graphene nanopatches, themetasurface reactance may be tuned from inductive to capacitive, as a functionof the relative kinetic inductance and the geometric patch capacitance, enablingthe possibility of effectively cloaking both dielectric and conducting objects atTHz frequencies with the same metasurface. We envision applications for low-observable nanostructures and efficient THz sensing, routing and detection.
3 Author to whom any correspondence should be addressed.
Content from this work may be used under the terms of the Creative Commons Attribution 3.0 licence.Any further distribution of this work must maintain attribution to the author(s) and the title of the work, journal
citation and DOI.
New Journal of Physics 15 (2013) 1230291367-2630/13/123029+12$33.00 © IOP Publishing Ltd and Deutsche Physikalische Gesellschaft
2
Contents
1. Introduction 22. Design of a graphene mantle cloak 43. Results and discussions 64. Conclusion 10Acknowledgments 11References 11
1. Introduction
Graphene is a single layer of sp2-bonded carbon atoms densely packed in a honeycomblattice [1, 2]. Ever since its discovery in 2004, graphene has attracted tremendous attentiondue to its stable thermal and mechanical properties and its special electronic properties, suchas high carrier mobility and Fermi velocity (vF
∼= 108 cm s−1), quantum Hall effect, largeoptical transparency, mechanical flexibility, among others [1–4]. Graphene is considered oneof the most promising material candidates for the next-generation of micro-/nano-electronicdevices [1–4] and for solar cells and flexible flat-panel displays [5].
This functional nanomaterial platform has been further enriched by the discovery of itsinherent plasmonic-like properties in the terahertz (THz) and infrared (IR) spectrum [6–14].Graphene plasmonics has become a rapidly emerging field because of the additionalpossibility, unique to graphene, of gate-tuning its optical transitions and the plasmonicresonance of massless Dirac fermions. Currently, graphene plasmonics has become the subjectof intensive research, with exciting applications for THz and IR tunable and switchablemetamaterials [14–18], filters and broadband polarizers [19], nano-antennas [20–22] andoptoelectronic devices [23], and with the ability to achieve ultrafast and broadband amplitudeand phase modulations.
Plasmonic effects have been also associated to cloaking and invisibility since the beginningof the interest in applying metamaterial concepts to scattering reduction [24], as the anomalouspolarization properties of these materials appear naturally suited to manipulate the scatteringof objects. Related to this possibility, we have recently proposed a mantle cloak consistingof a simple, homogeneous graphene monolayer [12], which is effective in the THz spectrum.We have demonstrated that a uniform graphene monolayer may enable a wideband-tunablescattering reduction for dielectric objects. Different from bulk metamaterial cloaks based ontransformation optics [25, 26], the physical principle behind this cloaking effect resides onscattering cancelation [12, 13, 24, 27–32], created by the surface current induced on thegraphene monolayer that may be tailored to radiate ‘anti-phase’ scattered fields [27–32]. Inaddition to extending the mantle cloaking technique [27] to THz frequencies, this graphenecloak offers the advantage of being frequency-reconfigurable, enabled by its tunable surfacereactance [12, 13]. Such a cloak may be used to potentially eliminate the cross-talk interferenceand noise in various THz sensing, imaging and communication systems [12, 13], as illustratedin figure 1(a). In this concept figure, we show a potential configuration in which a networkof sensors or detectors may significantly benefit from this technology by eliminating thecross-talk between neighboring elements operating in the THz spectrum. The proposed cloakallows receiving an impinging signal without necessarily creating significant scattering around
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
3
Figure 1. Schematic representation of (a) the concept, ‘cloaking a sensor’, forcross-talk-free and low-noise sensing and communication systems and networksin [20], and (b) the THz cloaking device based on the graphene-nanopatchmetasurface.
it [33], which may allow high-fidelity signal routing and reception for THz communications.Since conventional routing techniques are usually based on multiple dynamically assignedfrequency channels, the additional tunability of the proposed covers may be particularlyappealing.
One drawback of a graphene monolayer is that it is intrinsically inductive in the low-THzrange, and is therefore not able to cloak moderately sized conducting objects, which wouldrequire a capacitive surface impedance [27, 31]. To overcome this limitation, we propose in thefollowing a patterned graphene metasruface, which may significantly improve the performanceof the graphene cloak, as discussed in the following.
Recent progress in the growth and lithographic patterning of large-area epitaxialgraphene [2–4, 18] presents challenges and great opportunities for reconfigurable THz and IRmetamaterials and integrated plasmonic devices. It has been theoretically demonstrated that ametasurface formed by periodic arrays of subwavelength graphene nanopatches can possess adual inductive/capacitive surface impedance in the THz spectrum [16, 17], combining low-passand high-pass characteristics with potential applications for THz filters and polarizers [34–36].In this work, we investigate the performance of an atomically thin THz cloak made of a patternedgraphene monolayer (see figure 1(b)), which may achieve dramatic scattering reduction for bothdielectric and conducting rods, with larger flexibility compared to the homogeneous monolayerintroduced in [12]. We show that the surface impedance of such graphene metasurface hasa compact analytical expression, allowing us to readily design and optimize its geometry,dimensions and Fermi energy for effectively cloaking dielectric and/or conducting cylindricalobjects of choice with the same metasurface. More importantly, we show that the samemetasurface design may be employed to cloak drastically different objects, by properly tuningthe surface impedance through the proper weighing of the kinetic inductance of graphene andthe geometrical capacitance of the patterned surface.
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
4
2. Design of a graphene mantle cloak
The surface conductivity of a graphene sheet σs = σinter + σintra contains both semi-classicalintraband conductivity σintra and quantum-dynamical interband conductivity σinter. In the THzregion and below the interband transition threshold, hω < 2 |EF|, σintra dominates over σinter.Graphene’s intraband conductivity can be derived from the semiclassical Boltzmann transportequation, and in the local limit, applicable within the assumptions of this study, the conductivityis obtained as
σ ∼= σintra = ie2KBT
π h2(ω + iτ−1)ln
{2
[1 + cosh
(EF
KBT
)]}, (1)
where h is the reduced Plank constant, e is the electron charge, KB is the Boltzmann’s constant,EF is the Fermi energy, τ is the relaxation time related to impurities and defects in graphene andT is the temperature (here for convenience we assume a low-loss graphene with τ = 5 ps andT = 300 K; however, our additional studies show that the concepts outlined in the following mayalso be applied to graphene monolayers with smaller relaxation times). Throughout this study ane−iωt notation is adopted. For moderately doped graphene, |EF| � kBT (e.g. pristine grapheneintrinsically doped up to 0.25 eV by impurities [37]), and below the interband transitionthreshold, (1) reduces to a Drude-type dispersion
σintra ≈ ie2 EF/π h2
ω + iτ−1. (2)
From (2), we observe that a graphene monolayer has an inductive surface impedanceat low-THz: Zs = 1/σintra ≈ R − iωL , where L = π h2/e2 EF and R = τ−1L [9, 12–14].Moreover, different from conventional plasmonic materials, such as metals and heavily dopedsemiconductors, graphene’s conductivity can be controlled by shifting the electronic Fermilevels, which may be potentially tuned from −1 to 1 eV by chemical [38] or electronic doping[7, 8, 11].
Figure 1(b) shows the proposed graphene metasurface (a patterned graphenemicrotube [39]), wrapped around a dielectric or conducting rod. For a uniform plane wavenormally incident to the interface, the surface impedance of a planar array of graphenenanopatches has a simple yet accurate analytical expression [17, 40–42]
Zs = Rs − iXs =D
σs(D − g)+ i
π
2ωε0
(εr + 1
2
)D ln
[csc
(πg
2D
)] × ϕ (α) , (3)
where Rs is the surface resistance per unit cell related to the conduction losses, Xs is thesurface reactance per unit cell, D and g are the periodicity and gap size, respectively; α
is the incident angle, and ϕTM(α) = 1, ϕTE(θ) = 1 − sin2 α/(2εavg) are angular correlationfunctions corresponding to transverse magnetic (TM)- and transverse-electric (TE)-incidentpolarizations, respectively [31, 32, 41, 42]; εr is the relative permittivity of the dielectriccylinder or the spacer for the conducting cylinder, and ε0 is the background permittivity.The second term in (3) accounts for the capacitance per unit cell of the patch array CES =2Dπ
ε0(εr+1
2 ) ln[csc( πg2D )]ϕ(α) [31, 32, 41, 42]. The first term in (3) accounts for the tunable
kinetic inductance per unit cell LK =Im[1/σ ]
ω(1−g/D)=
π h2
e2 EF
11−g/D and the resistance per unit cell RG =
Re[1/σ ]1−g/D = LKτ−1, due to the intrinsic carrier scattering; RG and LK, tunable with EF, are in series
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
5
with the geometry-yielded capacitor CES. As a result, the surface impedance of this ‘one-atom-thick’ graphene metasurface may be modeled with a distributed RLC circuit model: Rs = RG
and Xs = ωLK − 1/ω CES. Since the kinetic inductance LK is tunable with EF, we note that thesurface reactance of the proposed graphene metasurface may be either capacitive or inductive,depending on the geometry, dimensions and Fermi energy. Therefore, a single metasurfacecan exhibit a highly controllable low-pass (capacitive) or high-pass (inductive) response. Thisproperty makes this geometry very different, and more appealing, than conventional metal-patchmetasurfaces in [17, 31, 32, 41, 42], which are fundamentally capacitive.
Consider now an infinite cylinder with radius a covered by a conformal graphenemetasruface cloak, illuminated by a normally incident TM plane wave (see figure 1(b)). Thisscenario is the case of most interest for scattering reduction purposes in this geometry, as longas the cross-section is comparable to the wavelength. For a conducting cylinder, a dielectricspacer with radius ac is necessary to avoid an electrical short. We first analyze the problemusing Lorenz–Mie scattering theory [43, 44], using a surface impedance boundary conditionbased on (3) at the surface of the graphene nanopatches. The scattering coefficients may beobtained by matching the tangential field components at the different boundaries, and may bewritten as [28, 29]
cTMn = −
PTMn
PTMn + iQTM
n
. (4)
The expressions for the nth order PTMn and QTM
n coefficients are found in [28, 29] asa function of the geometry and surface impedance. For an isotropic surface with negligiblecross-polarization coupling, the total scattering width, as a quantitative measure of the overallvisibility of the object at the frequency of interest, is given by [43, 44]
σs =4
k0
n=∞∑n=−∞
|cTMn |
2. (5)
In the quasi-static limit (i.e. k0a, k0ac � 1), the closed-form cloaking condition for adielectric cylinder under TM-polarized illumination can be derived as [28]
Xdiel∼=
2
ωaγ ε0(εr − 1), (6)
where γ = a/ac. On the other hand, for a conducting cylinder with moderate cross-sectioncovered by a thin spacer with relatively permittivity εr, the following cloaking condition isobtained, generalizing the results in [26]:
Xcond∼= −ωµ0a
γ 2− 1
γ (γ 2 + 1)−
ω3a3µ20(γ
2− 1)3[ε0 + εrε0(γ
2− 1)/2]
16γ 3(γ 2 + 1)3
∼= −ωµ0aγ 2
− 1
γ (γ 2 + 1), (7)
where µ0 is the permeability of background medium. It is interesting to note that the graphenemetasurface in figure 1(b) needs to have a dual inductive/capacitive nature to be able to holdfor (6) and (7). It is possible to achieve this property by balancing the geometric capacitanceof graphene patches with the intrinsic kinetic inductance of graphene, as we discuss in thefollowing.
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
6
Figure 2. Frequency dispersion of the surface reactance of a graphene monolayer(black-solid line) and the graphene metasurfaces I and II (red and blue solidlines). We also show the optimum surface reactance for cloaking a dielectriccylinder with a = λ0/8.4 and relative permittivity εr = 4 (orange-dashed-dottedline) and a conducting cylinder with a = λ0/12 covered by a thin spacer withthickness ac − a = λ0/28 and relative permittivity εr = 4 (green-dashed line); theoperating frequency is f0 = c/λ0 = 2.5 THz.
3. Results and discussions
Figure 2 shows the frequency dispersion of surface reactance for (i) a uniform graphene mono-layer with EF = 0.62 eV(black-solid line), (ii) a graphene-nanopatch metasurface (design I)with EF = 0.23 eV, D = 6.4 µm and g = 0.85 µm (red-solid line) and (iii) a graphene-nanopatch metasurface (design II) with EF = 0.3 eV, D = 7.6 µm and g = 0.5 µm (blue-solidline). In the plot we also show the optimal surface reactance, calculated using equation (4),to effectively cloak a dielectric cylinder with a = λ0/8.4 and relative permittivity εr = 4 (i.e.silicon dioxide, SiO2 or boron nitride, BN) (orange-dashed-dotted line), and using (7) for aconducting cylinder with a = λ0/12 covered by a spacer with thickness ac − a = λ0/28 andrelative permittivity εr = 4 (green-dotted line); here, we assume the operating frequency to bef0 = c/λ0 = 2.5 THz. It is observed from figure 2 that the optimum surface reactance valuesfor cloaking agree well with the quasi-static, approximate expressions Xdiel and Xcond in (6)and (7). Interestingly, their dispersions violates the Foster requirement of a positive slope∂ X (ω) /∂ω > 0 for low-loss passive metasurfaces, implying that broadband cloaking may notbe achieved with this or any other passive technology [45]. Still, targeting a specific designfrequency (in this case f0), it is possible to tune the desired surface reactance to cross therequired value given by the dashed curves, and therefore maximally suppress the scatteringwith a single metasurface.
For instance, consistent with equation (2), a graphene monolayer always displays a purelyinductive surface reactance [16], whose slope may be controlled to match the surface inductance215.37 � required to cloak the dielectric rod at f0, for EF = 0.62 eV (solid black line infigure 2). However, there is no value of carrier concentration or Fermi energy that may allow the
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
7
Figure 3. (a) Scattering width versus frequency for a dielectric rod (a =
14.28 µm and εr = 4) covered by a graphene monolayer and nanostructuredgraphene metasurfaces as in figure 2. Panel (b) is similar to (a), but for agraphene metasurface with same geometrical parameters (period and gap) asmetasurface I, but varying the Fermi energy.
solid black line, i.e. a uniform graphene monolayer, to meet the green dashed line representingthe required (capacitive) surface reactance to cloak a conducting object.
On the contrary, the surface reactance of metasurfaces I and II span capacitive and inductivevalues, and may therefore be used to cloak either a conducting or inductive object. In addition,the patch designs require comparatively a much lower carrier concentration to achieve theoptimal cloaking condition at the same frequency for the dielectric object. This is becausea uniform graphene monolayer inherently requires a large EF to achieve sufficiently lowsurface inductance (i.e. LK ∝ E−1
F ) to meet the orange dot-dashed line. This is particularlychallenging for higher frequencies, for which the optimal surface reactance gets lower andlower. However, the proposed graphene metasurface exploits the negative reactance providedby capacitive patches to compensate the high kinetic inductance of graphene with a lowcarrier concentration. As a result, the surface reactance may be tailored over a wide rangeof values, from capacitive to inductive, by tuning reasonably small values of Fermi energy.The dual capacitive/inductive graphene metasurface proposed here provides significantly addedflexibility in designing cloaking devices for dielectric/conducting objects at THz frequencies.
Figure 3(a) presents the calculated scattering width for the same dielectric cylinder as infigure 2, with and without the proposed graphene metasurface cloaks (graphene monolayer andnanostructured metasurfaces). It is seen that for all cloaking devices, the scattering width may besignificantly reduced at the operating frequency f0 = 2.5 THz. A graphene monolayer, however,has a larger bandwidth compared to graphene metasurfaces I and II, since its dispersion slope isless steep, and follows more closely the required surface impedance curve in figure 2 (orange-dashed-dotted line). However, nanostructured graphene metasurfaces require a significantlylower doping level and provide more design flexibility. Figure 3(b), similar to figure 3(a), refersto the case of graphene metasruface I varying the Fermi energy. It is observed that the scatteringwidth may be suppressed at different operating frequencies, tunable by shifting the Fermi energyof graphene nanopatches.
The same geometry may now also be applied to cloak the conducting rod by varyingthe geometry and/or Fermi energies. Figure 4(a) presents the calculated scattering width for
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
8
Figure 4. (a) Similar to figure 3(a), but for a conducting cylinder (a = 10 µm)isolated by a dielectric spacer (ac = 14.28 µm and εr = 4). Panel (b) is similar tofigure 4(a), but for a graphene metasurface with the same geometrical parameters(period and gap) as in metasurface III and different Fermi energies.
the same conducting cylinder as in figure 2, covered by a thin dielectric spacer, with andwithout a graphene metasurface cloak. We show the results for metasurface I, but with Fermienergy EF = 0.45 eV (labeled metasruface III). Similarly, we designed metasurface IV withEF = 0.6 eV, D = 6.2 µm and g = 0.5 µm to provide the same surface reactance at thedesign frequency. Obviously, both geometries allow strong scattering suppression, and similardispersion properties. The case of a graphene monolayer with EF = 0.45 eV is also presented infigure 4(a) for comparison. It is remarkable that the same metasurface geometry (designs I andIII) with different Fermi energies may be used to cloak either dielectric or conducting objectsat the same frequency ( f0 = 2.5 THz). On the contrary, a uniform graphene monolayer wouldnot be able to suppress any scattering for this conducting scenario, as seen in figure 4(a), sinceit cannot reach the optimal surface capacitance 108.28 � given by the dashed green line infigure 2.
Although the metasurfaces III and IV have different geometries and Fermi levels, theysupport the same operating frequency, showing the flexibility in design offered by the proposedgraphene metasruface geometry. Figure 4(b), similar to figure 4(a), refers to the case of agraphene metasurface with the same geometrical parameters (period and gap) as in metasurfaceI and III, but different Fermi energies. Again, it is seen that the scattering suppression isfrequency-tunable by tailoring the applied Fermi energy.
We validated our theory using commercial full-wave simulations based on CST MicrowaveStudio (finite-integral technique [46]). Figure 5(a) presents the scattering width of a dielectriccylinder with a = 14.28 µm, εr = 4 (figure 3(b)), with and without a graphene metasurfacecover with the same geometrical parameters as in metasurface I and EF = 0.37 eV (blue linein figure 3(b)). The numerical results (solid blue line/solid circles), obtained considering therealistic nanopatch geometry of the metasurface, are in excellent agreement with our analyticalformulation (solid red line/solid squares, equations (3)–(5)). Figures 5(b) and (c) respectivelypresent a time snapshot of the electric field distribution for the cloaked and uncloaked dielectriccylinder at the design frequency f0 = 3 THz. It is clear that, by covering the object with asuitable graphene metasurface, the wavefronts of electric field can be effectively restored, as ifthe object is not present. On the contrary, the electric field distribution is strongly disturbed inthe absence of the cloaking layer.
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
9
Figure 5. Numerical (solid blue line/solid circles) and analytical (solidred line/solid squares) comparison for: (a) scattering width of a dielectriccylinder with a = 14.28 µm and εr = 4, with and without (dashed grayline/open triangles) graphene metasurface cloak, and snapshots of electric fielddistributions for a cloaked (b) and an uncloaked (c) dielectric cylinder.
Figure 6 is similar to figure 5, but for the conducting rod considered above. Here, thegeometrical parameters of metasurfaces I and III are still used, but the Fermi energy is shiftedto 0.78 eV. It is observed in figure 6(a) that the scattering width is again significantly reducedat 3 THz. It is impressive how the same graphene metasurface may effectively cloak dielectricand conducting objects with similar dimensions at the same frequency by simply tuning itsFermi energy, proving the real-time reconfigurability of this cloaking approach. We note that, bysimply adjusting the geometry and doping level of graphene nanopatches, THz cloaking devicesmay be readily implemented for dielectric and conducting objects at the desired frequency, withinteresting potential for THz communications, sensing and photodetection.
Before concluding, we note that the polarization and incidence angle may both in principleaffect the cloaking effect. However, the first TM harmonic is the dominant scattering mechanismfor cylinders of moderate electrical cross section, and normal incidence produces the largesttotal scattering cross section [29, 30]. As a result, we have focused our designs and calculationson TM impinging radiation at normal incidence. We have shown in previous papers [12, 30]how the mantle cloaking technique applied to thin cylinders is indeed robust to variations inthe angle of incidence, and the results derived for infinite cylinders may be used to predict withgood approximation the response of finite elongated rods [47, 48]. In addition, the capacitanceyielded by the patch-array metasurface is independent of the incidence angle for TM waves, andthe kinetic inductance of graphene is independent of the incident angle for both polarizations.Therefore, the proposed graphene cloak is expected to be relatively insensitive to changes in
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
10
Figure 6. Similar to figure 5, but for a conducting cylinder (a = 10 µm) isolatedby a dielectric spacer (ac = 14.28 µm and εr = 4).
the excitation for thin dielectric and conducting cylinders. For thicker cylinders cross-polarizedcoupling between TM and TE scattering occurs at oblique incidence, and mantle cloaks mayrequire an anisotropic surface reactance to optimize the response, which goes beyond the scopeof this paper.
4. Conclusion
We have proposed the use of nanostructured graphene metasurface to realize an atomicallythin mantle cloak in the THz spectrum. Specifically, we have demonstrated that a graphene-nanopatch metasurface exhibits dual capacitive/inductive surface impedance, depending on therelative strength of graphene kinetic inductance and the geometric patch capacitance, which maybe effectively modeled in simple analytical terms. These peculiar features open exciting venuesto effectively cloak both dielectric and conducting rods with the same patterned metasurface,and reduce the requirements on required Fermi levels when using uniform graphene monolayers.The proposed metasurface is highly tunable, and may provide exciting venues in realizeultrathin, reconfigurable cloaking devices at THz frequencies, with potential applications in low-noise and cross-talk-free THz biomedical sensing and imaging systems, spectroscopy and THzcommunication and sensing networks, such as inter/intra-chip ultrafast links, indoor systemsand wireless health applications highlighted in [20]. The recent demonstration of a cloakedphotodetector based on scattering cancelation, put forward in [49], may be extended to THzfrequencies with this technology, with added tunability features uniquely stemming from thegraphene properties.
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
11
Acknowledgments
This work was supported in part by the AFOSR YIP award no. FA9550-11-1-0009, the DTRAYIP award no. HDTRA1-12-1-0022, the NSF CAREER award no. ECCS-0953311 and theNASA EPSCoR award NNX13AB31A
References
[1] Novoselov K S, Geim A K, Morozov S V, Jiang D, Zhang Y, Dubonos S V, Grigorieva I V and Firsov A A2004 Science 306 666–9
[2] Geim A K and Novoselov K S 2007 Nature Mater. 6 183–91[3] Neto A H C, Guinea F, Peres N M R, Novoselov K S and Geim A K 2009 Rev. Mod. Phys. 81 109–62[4] Lin Y M, Dimitrakopoulos C, Jenkins K A, Farmer D B, Chiu H Y, Grill A and Avouris Ph 2010 Science
327 662[5] Wang X, Zhi L and Mullen K 2008 Nano Lett. 8 323–7[6] Gusynin V P, Sharapov S G and Carbotte J P 2007 J. Phys.: Condens. Matter 19 026222[7] Hanson G W 2008 IEEE Trans. Antennas Propag. 56 747–57[8] Hanson G W 2008 J. Appl. Phys. 103 064302[9] Lovat G, Hanson G W, Araneo R and Burghignoli P 2013 Phys. Rev. B 87 115429
[10] Rana F 2008 IEEE Trans. Nanotechnol. 7 91–9[11] Chen J et al 2012 Nature 487 77–81[12] Chen P Y and Alu A 2011 ACS Nano 5 5855–63[13] Farhat M, Rockstuhl C and Bagci H 2013 Opt. Express 21 12592[14] Vakil A and Engheta N 2011 Science 332 1291–4[15] Koppens F H L, Chang D E and Garcia de Abajo F J 2011 Nano Lett. 11 3370–7[16] Kaipa C S R, Yakovlev A B, Hanson G W, Padooru Y R, Medina F and Mesa F 2012 Phys. Rev. B 85 245407[17] Padooru Y R, Yakovlev A B, Kaipa C S R, Hanson G W, Medina F and Mesa F 2013 Phys. Rev. B 87 115401[18] Ju L et al 2011 Nature Nanotechnol. 6 630–4[19] Bao Q, Zhang H, Wang B, Ni Z, Haley C, Lim Y X, Wang Y, Tang D Y and Loh K P 2011 Nature Photon.
5 411–5[20] Akyildiz I F and Jornet J M 2010 IEEE Wirel. Commun. Magn. 17 58–63[21] Carrasco E and Perruisseau-Carrier J 2013 IEEE Antennas Wirel. Propag. Lett. 12 253–6[22] Chen P Y, Argyropoulos C and Alu A 2013 IEEE Trans. Antennas Propag. 61 1528–37[23] Liu M, Yin X B, Ulin-Avila E, Geng B S, Zentgraf T, Ju L, Wang F and Zhang X 2011 Nature 474 64[24] Alu A and Engheta N 2005 Phys. Rev. E 72 016623[25] Pendry J B, Schurig D and Smith D R 2006 Science 312 1780–2[26] Schurig D, Mock J J, Justice B J, Cummer S A, Pendry J B, Starr A F and Smith D R 2006 Science 314 977–80[27] Alu A 2009 Phys. Rev. B 80 245115[28] Chen P Y and Alu A 2011 Phys. Rev. B 84 205110[29] Chen P Y, Soric J and Alu A 2012 Adv. Mater. 24 OP281–OP304[30] Soric J C, Chen P Y, Kerkhoff A, Rainwater D, Melin K and Alu A 2013 New J. Phys. 15 033037[31] Padooru Y R, Yakovlev A B, Chen P Y and Alu A 2012 J. Appl. Phys. 112 104902[32] Padooru Y R, Yakovlev A B, Chen P Y and Alu A 2012 J. Appl. Phys. 112 034907[33] Alu A and Engheta N 2009 Phys. Rev. Lett. 102 233901[34] Fallahi A and Perruisseau-Carrier J 2012 Phys. Rev. B 86 195408[35] Nikitin A Yu, Guinea F and Martin-Moreno L 2012 Appl. Phys. Lett. 101 151119[36] Chen P Y and Alu A 2012 Integrated infrared nanodevices based on graphene monolayers IEEE Antennas
and Propagation Symp. (Chicago, IL, 8–14 July) doi:10.1109/APS.2012.6349215[37] Berciaud S, Ryu S, Brus L E and Heinz T F 2009 Nano Lett. 9 346–52
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)
12
[38] Chuang F T, Chen P Y, Cheng T C, Chien C H and Li B J 2007 Nanotechnology 18 395702[39] Hu J Q et al 2004 Adv. Mater. 16 153–6[40] Whitbourn L B and Compton R C 1985 Appl. Opt. 24 217–20[41] Luukkonen O, Simovski C, Granet G, Goussetis G, Lioubtchenko D, Raisanen A V and Treyakov S A 2008
IEEE Trans. Antennas Propag. 56 1624–32[42] Padooru Y R, Yakovlev A B, Kaipa C S R, Medina F and Mesa F 2011 Phys. Rev. B 84 035108[43] Bohren C F and Huffman D R 1998 Absorption and Scattering of Light by Small Particles (New York: Wiley)[44] Papas C H 1988 Theory of Electromagnetic Wave Propagation (New York: Dover)[45] Chen P Y, Argyropoulos C and Alu A 2013 arXiv:1306.5835[46] CST Microwave Studio 2012 www.cst.com[47] Rainwater D, Kerkhoff A, Melin K, Soric J C, Moreno G and Alu A 2012 New J. Phys. 14 013054[48] Alu A, Rainwater D and Kerkhoff A 2010 New J. Phys. 12 103028[49] Fan P, Chettiar U K, Cao L, Afshinmanesh F, Engheta N and Brongersma M L 2012 Nature Photon. 6 380–5
New Journal of Physics 15 (2013) 123029 (http://www.njp.org/)